# Electronic Supplementary Material (ESI) for Inorganic Chemistry Frontiers.
# This journal is © the Partner Organisations 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_aaa
_database_code_depnum_ccdc_archive 'CCDC 2158241'
loop_
_audit_author_name
_audit_author_address
'mengran sun'
;University of Chinese Academy of Sciences 
China
;
_audit_update_record             
;
2022-03-14 deposited with the CCDC.	2022-05-03 downloaded from the CCDC.
;
_audit_creation_date             2021-11-09
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'Ba6 Ge2 In2 Te15'
_chemical_formula_sum            'Ba6 Ge2 In2 Te15'
_chemical_formula_weight         3112.86
_chemical_melting_point          1053
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ge Ge 0.1547 1.8001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
In In -0.7276 1.3100 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 1 21/c 1'
_space_group_name_Hall           '-P 2ybc'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'

_cell_length_a                   9.6201(6)
_cell_length_b                   13.4225(7)
_cell_length_c                   27.5845(16)
_cell_angle_alpha                90
_cell_angle_beta                 92.469(2)
_cell_angle_gamma                90
_cell_volume                     3558.6(4)
_cell_formula_units_Z            4
_cell_measurement_reflns_used    7764
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      30.5
_cell_measurement_theta_min      3.09
_shelx_estimated_absorpt_T_max   ?
_shelx_estimated_absorpt_T_min   ?
_exptl_absorpt_coefficient_mu    21.505
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_type   none
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'metallic dark black'
_exptl_crystal_colour_lustre     metallic
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    5.810
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       plate
_exptl_crystal_F_000             5112
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0852
_diffrn_reflns_av_unetI/netI     0.0734
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       39
_diffrn_reflns_limit_l_min       -39
_diffrn_reflns_number            73611
_diffrn_reflns_point_group_measured_fraction_full 0.999
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         30.529
_diffrn_reflns_theta_min         1.478
_diffrn_ambient_temperature      296
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                7764
_reflns_number_total             10847
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'ShelXL (Sheldrick, 2015)'
_computing_structure_solution    'ShelXT (Sheldrick, 2015)'
_refine_diff_density_max         2.627
_refine_diff_density_min         -2.630
_refine_diff_density_rms         0.601
_refine_ls_extinction_coef       0.000427(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2014/7 (Sheldrick 2014'
_refine_ls_goodness_of_fit_ref   1.080
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     227
_refine_ls_number_reflns         10847
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0856
_refine_ls_R_factor_gt           0.0512
_refine_ls_restrained_S_all      1.080
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0076P)²+99.7822P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0804
_refine_ls_wR_factor_ref         0.0896
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ba1 Ba 0.50162(7) 0.31589(5) 0.37092(3) 0.01360(15) Uani 1 1 d . . . . .
Ba2 Ba 0.50750(7) 0.45835(5) 0.20046(3) 0.01224(15) Uani 1 1 d . . . . .
Ba3 Ba 1.00677(7) 0.31192(5) 0.37388(3) 0.01281(15) Uani 1 1 d . . . . .
Ba4 Ba 0.99171(7) 0.94826(5) 0.30258(3) 0.01180(14) Uani 1 1 d . . . . .
Ba5 Ba 0.99470(7) 0.80865(5) 0.46400(3) 0.01170(14) Uani 1 1 d . . . . .
Ba6 Ba 0.49139(7) 0.81112(5) 0.46628(3) 0.01193(14) Uani 1 1 d . . . . .
In1 In 0.74904(9) 0.52780(6) 0.46253(3) 0.01425(18) Uani 1 1 d . . . . .
In2 In 0.23407(9) 0.64542(6) 0.31143(3) 0.01541(19) Uani 1 1 d . . . . .
Ge1 Ge 0.63192(13) 0.67377(9) 0.34071(5) 0.0117(3) Uani 1 1 d . . . . .
Ge2 Ge 0.83953(13) 0.58248(9) 0.32255(5) 0.0119(3) Uani 1 1 d . . . . .
Te1 Te 0.50292(8) 0.57351(5) 0.40536(3) 0.01315(16) Uani 1 1 d . . . . .
Te2 Te 0.48042(8) 0.69816(5) 0.26086(3) 0.01253(16) Uani 1 1 d . . . . .
Te3 Te 0.72733(8) 0.83785(5) 0.37475(3) 0.01099(15) Uani 1 1 d . . . . .
Te4 Te 0.76619(8) 0.41020(5) 0.29036(3) 0.01204(16) Uani 1 1 d . . . . .
Te5 Te 0.98183(8) 0.56997(5) 0.40451(3) 0.01298(16) Uani 1 1 d . . . . .
Te6 Te 0.74510(8) 0.67208(6) 0.53243(3) 0.01396(16) Uani 1 1 d . . . . .
Te7 Te 0.75390(8) 0.32458(5) 0.46745(3) 0.01348(16) Uani 1 1 d . . . . .
Te8 Te 0.24732(8) 0.44115(5) 0.29811(3) 0.01319(16) Uani 1 1 d . . . . .
Te9 Te -0.02882(8) 0.68674(5) 0.26005(3) 0.01273(16) Uani 1 1 d . . . . .
Te10 Te 0.23999(8) 0.81123(5) 0.37087(3) 0.01192(16) Uani 1 1 d . . . . .
Te11 Te 0.74538(8) 0.87135(5) 0.65755(3) 0.01410(17) Uani 1 1 d . . . . .
Te12 Te 0.56614(8) 0.93332(5) 0.58120(3) 0.01305(16) Uani 1 1 d . . . . .
Te13 Te 0.75185(8) 0.99923(5) 0.50246(3) 0.01525(17) Uani 1 1 d . . . . .
Te14 Te 0.93799(8) 1.06481(5) 0.41953(3) 0.01273(16) Uani 1 1 d . . . . .
Te15 Te 0.75808(8) 1.12883(5) 0.34334(3) 0.01325(16) Uani 1 1 d . . . . .









_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ba5 Ba6 4.7761(10) 1_655 ?
Ba5 Ba3 4.7565(10) 3_766 ?
Ba5 Ba4 4.8300(10) . ?
Ba5 Te3 3.5050(10) . ?
Ba5 Te10 3.5625(11) 1_655 ?
Ba5 Te13 3.6409(10) 3_776 ?
Ba5 Te13 3.6524(10) . ?
Ba5 Te14 3.6668(10) 3_776 ?
Ba5 Te14 3.6832(10) . ?
Ba5 Te5 3.5993(10) . ?
Ba5 Te7 3.4969(10) 3_766 ?
Ba5 Te6 3.6165(11) . ?
Ba1 Ba6 4.8014(10) 3_666 ?
Ba1 Ba3 4.7651(11) 1_455 ?
Ba1 Te15 3.6237(10) 1_545 ?
Ba1 Te11 3.5240(10) 3_666 ?
Ba1 Te8 3.5245(10) . ?
Ba1 Te4 3.6750(11) . ?
Ba1 Te1 3.5859(10) . ?
Ba1 Te12 3.6650(10) 3_666 ?
Ba1 Te2 3.9742(11) 2_645 ?
Ba1 Te7 3.5266(11) . ?
Ba1 Te6 3.6487(11) 3_666 ?
Ba6 Ba5 4.7761(10) 1_455 ?
Ba6 Ba1 4.8014(10) 3_666 ?
Ba6 Te3 3.4854(11) . ?
Ba6 Te10 3.4966(10) . ?
Ba6 Te13 3.5880(10) 3_676 ?
Ba6 Te13 3.6653(10) . ?
Ba6 Te1 3.6087(10) . ?
Ba6 Te12 3.6141(10) . ?
Ba6 Te12 3.7049(10) 3_676 ?
Ba6 Te7 3.5495(10) 3_666 ?
Ba6 Te6 3.5194(10) . ?
Ba3 Ba5 4.7565(10) 3_766 ?
Ba3 Ba1 4.7650(11) 1_655 ?
Ba3 Te15 3.5069(10) 1_545 ?
Ba3 Te11 3.5590(10) 3_766 ?
Ba3 Te8 3.6260(11) 1_655 ?
Ba3 Te4 3.4561(10) . ?
Ba3 Te14 3.6190(10) 1_545 ?
Ba3 Te5 3.5758(10) . ?
Ba3 Te7 3.6263(11) . ?
Ba3 Te6 3.4485(11) 3_766 ?
Ba2 Ba4 4.8015(10) 2_645 ?
Ba2 Ba4 4.8239(10) 2_745 ?
Ba2 Te3 3.4087(10) 2_645 ?
Ba2 Te15 3.5996(10) 2_645 ?
Ba2 Te11 3.4779(10) 4_575 ?
Ba2 Te10 3.7527(10) 2_645 ?
Ba2 Te8 3.7624(11) . ?
Ba2 Te4 3.4970(10) . ?
Ba2 Te12 3.6624(11) 4_575 ?
Ba2 Te2 3.6390(10) . ?
Ba2 Te2 3.6522(10) 2_645 ?
Ba4 Ba2 4.8015(10) 2_655 ?
Ba4 Ba2 4.8239(10) 2_755 ?
Ba4 Te9 3.7038(10) 1_655 ?
Ba4 Te9 3.6621(10) 2_655 ?
Ba4 Te3 3.6145(10) . ?
Ba4 Te15 3.5225(10) . ?
Ba4 Te11 3.6373(10) 3_776 ?
Ba4 Te10 3.4998(10) 1_655 ?
Ba4 Te8 3.5301(10) 2_655 ?
Ba4 Te4 3.5738(11) 2_755 ?
Ba4 Te14 3.6421(10) . ?
Te9 Ba4 3.7037(10) 1_455 ?
Te9 Ba4 3.6622(10) 2_645 ?
Te9 In2 2.8989(12) . ?
Te9 Ge2 2.5927(15) 1_455 ?
Te3 Ba2 3.4087(10) 2_655 ?
Te3 Ge1 2.5495(14) . ?
Te15 Ba1 3.6237(10) 1_565 ?
Te15 Ba3 3.5069(10) 1_565 ?
Te15 Ba2 3.5996(10) 2_655 ?
Te15 Te14 2.7996(11) . ?
Te11 Ba1 3.5239(10) 3_666 ?
Te11 Ba3 3.5589(10) 3_766 ?
Te11 Ba2 3.4779(10) 4_576 ?
Te11 Ba4 3.6373(10) 3_776 ?
Te11 Te12 2.7905(11) . ?
Te10 Ba5 3.5625(11) 1_455 ?
Te10 Ba2 3.7527(11) 2_655 ?
Te10 Ba4 3.4998(10) 1_455 ?
Te10 In2 2.7635(11) . ?
Te8 Ba3 3.6261(11) 1_455 ?
Te8 Ba4 3.5301(10) 2_645 ?
Te8 In2 2.7699(11) . ?
Te4 Ba4 3.5739(11) 2_745 ?
Te4 Ge2 2.5651(14) . ?
Te13 Ba5 3.6410(10) 3_776 ?
Te13 Ba6 3.5880(10) 3_676 ?
Te13 Te14 3.0931(12) . ?
Te13 Te12 3.0045(12) . ?
Te1 In1 2.8545(12) . ?
Te1 Ge1 2.5927(15) . ?
Te14 Ba5 3.6670(10) 3_776 ?
Te14 Ba3 3.6190(10) 1_565 ?
Te5 In1 2.8646(12) . ?
Te5 Ge2 2.5975(15) . ?
Te12 Ba1 3.6650(10) 3_666 ?
Te12 Ba6 3.7049(10) 3_676 ?
Te12 Ba2 3.6623(11) 4_576 ?
Te2 Ba1 3.9743(11) 2_655 ?
Te2 Ba2 3.6522(10) 2_655 ?
Te2 In2 2.8893(12) . ?
Te2 Ge1 2.6088(15) . ?
Te7 Ba5 3.4970(10) 3_766 ?
Te7 Ba6 3.5496(10) 3_666 ?
Te7 In1 2.7314(11) . ?
Te6 Ba1 3.6487(11) 3_666 ?
Te6 Ba3 3.4486(10) 3_766 ?
Te6 In1 2.7342(11) . ?
Ge2 Te9 2.5927(15) 1_655 ?
Ge2 Ge1 2.4141(17) . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Ba6 Ba5 Ba4 88.603(17) 1_655 . ?
Ba3 Ba5 Ba6 91.920(17) 3_766 1_655 ?
Ba3 Ba5 Ba4 177.02(2) 3_766 . ?
Te3 Ba5 Ba6 135.39(2) . 1_655 ?
Te3 Ba5 Ba3 131.81(2) . 3_766 ?
Te3 Ba5 Ba4 48.243(17) . . ?
Te3 Ba5 Te10 88.92(2) . 1_655 ?
Te3 Ba5 Te13 124.23(3) . 3_776 ?
Te3 Ba5 Te13 70.52(2) . . ?
Te3 Ba5 Te14 131.31(3) . 3_776 ?
Te3 Ba5 Te14 64.41(2) . . ?
Te3 Ba5 Te5 76.67(2) . . ?
Te3 Ba5 Te6 86.54(2) . . ?
Te10 Ba5 Ba6 46.843(17) 1_655 1_655 ?
Te10 Ba5 Ba3 135.25(2) 1_655 3_766 ?
Te10 Ba5 Ba4 46.310(17) 1_655 . ?
Te10 Ba5 Te13 130.88(3) 1_655 . ?
Te10 Ba5 Te13 73.69(2) 1_655 3_776 ?
Te10 Ba5 Te14 121.99(3) 1_655 3_776 ?
Te10 Ba5 Te14 81.02(2) 1_655 . ?
Te10 Ba5 Te5 71.98(2) 1_655 . ?
Te10 Ba5 Te6 148.94(3) 1_655 . ?
Te13 Ba5 Ba6 130.05(2) . 1_655 ?
Te13 Ba5 Ba6 48.173(17) 3_776 1_655 ?
Te13 Ba5 Ba3 86.41(2) . 3_766 ?
Te13 Ba5 Ba3 91.78(2) 3_776 3_766 ?
Te13 Ba5 Ba4 91.01(2) . . ?
Te13 Ba5 Ba4 86.38(2) 3_776 . ?
Te13 Ba5 Te13 81.95(2) 3_776 . ?
Te13 Ba5 Te14 60.76(2) 3_776 . ?
Te13 Ba5 Te14 50.08(2) 3_776 3_776 ?
Te13 Ba5 Te14 60.80(2) . 3_776 ?
Te13 Ba5 Te14 49.88(2) . . ?
Te14 Ba5 Ba6 97.57(2) . 1_655 ?
Te14 Ba5 Ba6 81.17(2) 3_776 1_655 ?
Te14 Ba5 Ba3 48.810(17) 3_776 3_766 ?
Te14 Ba5 Ba3 128.64(2) . 3_766 ?
Te14 Ba5 Ba4 48.384(16) . . ?
Te14 Ba5 Ba4 128.45(2) 3_776 . ?
Te14 Ba5 Te14 82.96(2) 3_776 . ?
Te5 Ba5 Ba6 91.54(2) . 1_655 ?
Te5 Ba5 Ba3 97.15(2) . 3_766 ?
Te5 Ba5 Ba4 85.77(2) . . ?
Te5 Ba5 Te13 138.24(3) . . ?
Te5 Ba5 Te13 139.09(3) . 3_776 ?
Te5 Ba5 Te14 132.63(3) . . ?
Te5 Ba5 Te14 144.40(3) . 3_776 ?
Te5 Ba5 Te6 77.07(2) . . ?
Te7 Ba5 Ba6 47.795(18) 3_766 1_655 ?
Te7 Ba5 Ba3 49.279(18) 3_766 3_766 ?
Te7 Ba5 Ba4 132.33(2) 3_766 . ?
Te7 Ba5 Te3 155.02(3) 3_766 . ?
Te7 Ba5 Te10 86.03(2) 3_766 1_655 ?
Te7 Ba5 Te13 129.59(3) 3_766 . ?
Te7 Ba5 Te13 77.57(2) 3_766 3_776 ?
Te7 Ba5 Te14 70.81(2) 3_766 3_776 ?
Te7 Ba5 Te14 138.29(3) 3_766 . ?
Te7 Ba5 Te5 78.51(2) 3_766 . ?
Te7 Ba5 Te6 85.29(2) 3_766 . ?
Te6 Ba5 Ba6 133.08(2) . 1_655 ?
Te6 Ba5 Ba3 46.204(17) . 3_766 ?
Te6 Ba5 Ba4 134.43(2) . . ?
Te6 Ba5 Te13 75.88(2) . . ?
Te6 Ba5 Te13 132.75(3) . 3_776 ?
Te6 Ba5 Te14 82.74(2) . 3_776 ?
Te6 Ba5 Te14 123.70(3) . . ?
Ba3 Ba1 Ba6 87.349(17) 1_455 3_666 ?
Te15 Ba1 Ba6 88.17(2) 1_545 3_666 ?
Te15 Ba1 Ba3 133.28(2) 1_545 1_455 ?
Te15 Ba1 Te4 67.43(2) 1_545 . ?
Te15 Ba1 Te12 64.95(2) 1_545 3_666 ?
Te15 Ba1 Te2 58.38(2) 1_545 2_645 ?
Te15 Ba1 Te6 130.86(3) 1_545 3_666 ?
Te11 Ba1 Ba6 86.41(2) 3_666 3_666 ?
Te11 Ba1 Ba3 48.032(17) 3_666 1_455 ?
Te11 Ba1 Te15 85.28(2) 3_666 1_545 ?
Te11 Ba1 Te8 76.61(2) 3_666 . ?
Te11 Ba1 Te4 126.07(3) 3_666 . ?
Te11 Ba1 Te1 137.85(3) 3_666 . ?
Te11 Ba1 Te12 45.63(2) 3_666 3_666 ?
Te11 Ba1 Te2 64.41(2) 3_666 2_645 ?
Te11 Ba1 Te7 128.85(3) 3_666 . ?
Te11 Ba1 Te6 74.97(2) 3_666 3_666 ?
Te8 Ba1 Ba6 133.14(2) . 3_666 ?
Te8 Ba1 Ba3 49.128(18) . 1_455 ?
Te8 Ba1 Te15 132.30(3) . 1_545 ?
Te8 Ba1 Te4 88.45(2) . . ?
Te8 Ba1 Te1 71.66(2) . . ?
Te8 Ba1 Te12 120.72(3) . 3_666 ?
Te8 Ba1 Te2 74.04(2) . 2_645 ?
Te8 Ba1 Te7 148.50(3) . . ?
Te8 Ba1 Te6 86.44(2) . 3_666 ?
Te4 Ba1 Ba6 134.89(2) . 3_666 ?
Te4 Ba1 Ba3 137.11(2) . 1_455 ?
Te4 Ba1 Te2 61.67(2) . 2_645 ?
Te1 Ba1 Ba6 95.44(2) . 3_666 ?
Te1 Ba1 Ba3 89.90(2) . 1_455 ?
Te1 Ba1 Te15 136.81(3) . 1_545 ?
Te1 Ba1 Te4 80.41(2) . . ?
Te1 Ba1 Te12 141.56(3) . 3_666 ?
Te1 Ba1 Te2 128.75(3) . 2_645 ?
Te1 Ba1 Te6 76.04(2) . 3_666 ?
Te12 Ba1 Ba6 48.275(17) 3_666 3_666 ?
Te12 Ba1 Ba3 77.895(19) 3_666 1_455 ?
Te12 Ba1 Te4 132.13(3) 3_666 . ?
Te12 Ba1 Te2 88.97(2) 3_666 2_645 ?
Te2 Ba1 Ba6 135.64(2) 2_645 3_666 ?
Te2 Ba1 Ba3 95.39(2) 2_645 1_455 ?
Te7 Ba1 Ba6 47.474(17) . 3_666 ?
Te7 Ba1 Ba3 130.01(2) . 1_455 ?
Te7 Ba1 Te15 74.27(2) . 1_545 ?
Te7 Ba1 Te4 88.46(2) . . ?
Te7 Ba1 Te1 76.92(2) . . ?
Te7 Ba1 Te12 83.42(2) . 3_666 ?
Te7 Ba1 Te2 130.40(3) . 2_645 ?
Te7 Ba1 Te6 83.97(2) . 3_666 ?
Te6 Ba1 Ba6 46.811(17) 3_666 3_666 ?
Te6 Ba1 Ba3 46.065(17) 3_666 1_455 ?
Te6 Ba1 Te4 156.33(3) 3_666 . ?
Te6 Ba1 Te12 69.25(2) 3_666 3_666 ?
Te6 Ba1 Te2 137.83(3) 3_666 2_645 ?
Ba5 Ba6 Ba1 89.056(17) 1_455 3_666 ?
Te3 Ba6 Ba5 132.34(2) . 1_455 ?
Te3 Ba6 Ba1 136.95(2) . 3_666 ?
Te3 Ba6 Te10 84.59(2) . . ?
Te3 Ba6 Te13 70.58(2) . . ?
Te3 Ba6 Te13 123.57(3) . 3_676 ?
Te3 Ba6 Te1 73.72(2) . . ?
Te3 Ba6 Te12 118.52(3) . . ?
Te3 Ba6 Te12 74.97(2) . 3_676 ?
Te3 Ba6 Te7 153.38(3) . 3_666 ?
Te3 Ba6 Te6 88.36(2) . . ?
Te10 Ba6 Ba5 48.008(18) . 1_455 ?
Te10 Ba6 Ba1 133.27(2) . 3_666 ?
Te10 Ba6 Te13 75.14(2) . 3_676 ?
Te10 Ba6 Te13 130.33(3) . . ?
Te10 Ba6 Te1 71.58(2) . . ?
Te10 Ba6 Te12 139.91(3) . . ?
Te10 Ba6 Te12 69.24(2) . 3_676 ?
Te10 Ba6 Te7 86.23(2) . 3_666 ?
Te10 Ba6 Te6 146.33(3) . . ?
Te13 Ba6 Ba5 132.86(2) . 1_455 ?
Te13 Ba6 Ba5 49.127(17) 3_676 1_455 ?
Te13 Ba6 Ba1 90.58(2) 3_676 3_666 ?
Te13 Ba6 Ba1 90.46(2) . 3_666 ?
Te13 Ba6 Te13 83.74(2) 3_676 . ?
Te13 Ba6 Te1 140.57(3) 3_676 . ?
Te13 Ba6 Te12 64.80(2) 3_676 . ?
Te13 Ba6 Te12 48.63(2) 3_676 3_676 ?
Te13 Ba6 Te12 63.15(2) . 3_676 ?
Te1 Ba6 Ba5 92.21(2) . 1_455 ?
Te1 Ba6 Ba1 97.02(2) . 3_666 ?
Te1 Ba6 Te13 134.53(3) . . ?
Te1 Ba6 Te12 143.19(3) . . ?
Te1 Ba6 Te12 131.36(3) . 3_676 ?
Te12 Ba6 Ba5 82.394(19) 3_676 1_455 ?
Te12 Ba6 Ba5 100.13(2) . 1_455 ?
Te12 Ba6 Ba1 130.94(2) 3_676 3_666 ?
Te12 Ba6 Ba1 49.188(17) . 3_666 ?
Te12 Ba6 Te13 48.75(2) . . ?
Te12 Ba6 Te12 84.89(2) . 3_676 ?
Te7 Ba6 Ba5 46.866(17) 3_666 1_455 ?
Te7 Ba6 Ba1 47.072(18) 3_666 3_666 ?
Te7 Ba6 Te13 77.60(2) 3_666 3_676 ?
Te7 Ba6 Te13 132.46(3) 3_666 . ?
Te7 Ba6 Te1 79.68(2) 3_666 . ?
Te7 Ba6 Te12 83.84(2) 3_666 . ?
Te7 Ba6 Te12 124.38(3) 3_666 3_676 ?
Te6 Ba6 Ba5 132.39(2) . 1_455 ?
Te6 Ba6 Ba1 49.103(18) . 3_666 ?
Te6 Ba6 Te13 134.14(3) . 3_676 ?
Te6 Ba6 Te13 76.90(2) . . ?
Te6 Ba6 Te1 74.83(2) . . ?
Te6 Ba6 Te12 71.25(2) . . ?
Te6 Ba6 Te12 139.81(3) . 3_676 ?
Te6 Ba6 Te7 85.55(2) . 3_666 ?
Ba5 Ba3 Ba1 93.631(17) 3_766 1_655 ?
Te15 Ba3 Ba5 87.58(2) 1_545 3_766 ?
Te15 Ba3 Ba1 132.49(2) 1_545 1_655 ?
Te15 Ba3 Te11 85.09(2) 1_545 3_766 ?
Te15 Ba3 Te8 129.98(3) 1_545 1_655 ?
Te15 Ba3 Te14 46.23(2) 1_545 1_545 ?
Te15 Ba3 Te5 133.12(3) 1_545 . ?
Te15 Ba3 Te7 74.47(2) 1_545 . ?
Te11 Ba3 Ba5 91.32(2) 3_766 3_766 ?
Te11 Ba3 Ba1 47.409(17) 3_766 1_655 ?
Te11 Ba3 Te8 74.89(2) 3_766 1_655 ?
Te11 Ba3 Te14 65.53(2) 3_766 1_545 ?
Te11 Ba3 Te5 141.22(3) 3_766 . ?
Te11 Ba3 Te7 133.06(3) 3_766 . ?
Te8 Ba3 Ba5 137.09(2) 1_655 3_766 ?
Te8 Ba3 Ba1 47.305(17) 1_655 1_655 ?
Te8 Ba3 Te7 148.45(3) 1_655 . ?
Te4 Ba3 Ba5 136.68(2) . 3_766 ?
Te4 Ba3 Ba1 128.69(2) . 1_655 ?
Te4 Ba3 Te15 71.16(2) . 1_545 ?
Te4 Ba3 Te11 122.54(3) . 3_766 ?
Te4 Ba3 Te8 81.89(2) . 1_655 ?
Te4 Ba3 Te14 117.04(3) . 1_545 ?
Te4 Ba3 Te5 74.81(2) . . ?
Te4 Ba3 Te7 90.35(2) . . ?
Te14 Ba3 Ba5 49.682(17) 1_545 3_766 ?
Te14 Ba3 Ba1 102.36(2) 1_545 1_655 ?
Te14 Ba3 Te8 140.33(3) 1_545 1_655 ?
Te14 Ba3 Te7 69.94(2) 1_545 . ?
Te5 Ba3 Ba5 96.00(2) . 3_766 ?
Te5 Ba3 Ba1 94.04(2) . 1_655 ?
Te5 Ba3 Te8 73.97(2) . 1_655 ?
Te5 Ba3 Te14 142.22(3) . 1_545 ?
Te5 Ba3 Te7 74.48(2) . . ?
Te7 Ba3 Ba5 46.957(17) . 3_766 ?
Te7 Ba3 Ba1 135.48(2) . 1_655 ?
Te6 Ba3 Ba5 49.197(18) 3_766 3_766 ?
Te6 Ba3 Ba1 49.635(18) 3_766 1_655 ?
Te6 Ba3 Te15 131.81(3) 3_766 1_545 ?
Te6 Ba3 Te11 77.07(2) 3_766 3_766 ?
Te6 Ba3 Te8 87.93(2) 3_766 1_655 ?
Te6 Ba3 Te4 153.88(3) 3_766 . ?
Te6 Ba3 Te14 85.83(2) 3_766 1_545 ?
Te6 Ba3 Te5 79.28(2) 3_766 . ?
Te6 Ba3 Te7 85.84(2) 3_766 . ?
Ba4 Ba2 Ba4 176.21(2) 2_645 2_745 ?
Te3 Ba2 Ba4 127.76(2) 2_645 2_745 ?
Te3 Ba2 Ba4 48.688(17) 2_645 2_645 ?
Te3 Ba2 Te15 69.83(2) 2_645 2_645 ?
Te3 Ba2 Te11 122.23(3) 2_645 4_575 ?
Te3 Ba2 Te10 81.85(2) 2_645 2_645 ?
Te3 Ba2 Te8 87.86(2) 2_645 . ?
Te3 Ba2 Te4 140.95(3) 2_645 . ?
Te3 Ba2 Te12 76.44(2) 2_645 4_575 ?
Te3 Ba2 Te2 129.77(3) 2_645 . ?
Te3 Ba2 Te2 74.69(2) 2_645 2_645 ?
Te15 Ba2 Ba4 46.935(17) 2_645 2_645 ?
Te15 Ba2 Ba4 134.99(2) 2_645 2_745 ?
Te15 Ba2 Te10 128.66(3) 2_645 2_645 ?
Te15 Ba2 Te8 78.16(2) 2_645 . ?
Te15 Ba2 Te12 65.21(2) 2_645 4_575 ?
Te15 Ba2 Te2 61.81(2) 2_645 . ?
Te15 Ba2 Te2 135.98(3) 2_645 2_645 ?
Te11 Ba2 Ba4 48.722(17) 4_575 2_745 ?
Te11 Ba2 Ba4 133.23(2) 4_575 2_645 ?
Te11 Ba2 Te15 86.32(2) 4_575 2_645 ?
Te11 Ba2 Te10 73.57(2) 4_575 2_645 ?
Te11 Ba2 Te8 138.74(3) 4_575 . ?
Te11 Ba2 Te4 84.51(2) 4_575 . ?
Te11 Ba2 Te12 45.92(2) 4_575 4_575 ?
Te11 Ba2 Te2 68.63(2) 4_575 . ?
Te11 Ba2 Te2 135.63(3) 4_575 2_645 ?
Te10 Ba2 Ba4 130.21(2) 2_645 2_645 ?
Te10 Ba2 Ba4 46.101(16) 2_645 2_745 ?
Te10 Ba2 Te8 143.97(2) 2_645 . ?
Te8 Ba2 Ba4 134.94(2) . 2_745 ?
Te8 Ba2 Ba4 46.766(16) . 2_645 ?
Te4 Ba2 Ba4 47.654(17) . 2_745 ?
Te4 Ba2 Ba4 133.46(2) . 2_645 ?
Te4 Ba2 Te15 145.96(3) . 2_645 ?
Te4 Ba2 Te10 79.49(2) . 2_645 ?
Te4 Ba2 Te8 87.48(2) . . ?
Te4 Ba2 Te12 125.30(3) . 4_575 ?
Te4 Ba2 Te2 84.35(2) . . ?
Te4 Ba2 Te2 66.63(2) . 2_645 ?
Te12 Ba2 Ba4 78.64(2) 4_575 2_745 ?
Te12 Ba2 Ba4 100.85(2) 4_575 2_645 ?
Te12 Ba2 Te10 67.03(2) 4_575 2_645 ?
Te12 Ba2 Te8 143.17(3) 4_575 . ?
Te2 Ba2 Ba4 87.65(2) 2_645 2_745 ?
Te2 Ba2 Ba4 86.66(2) . 2_645 ?
Te2 Ba2 Ba4 89.85(2) 2_645 2_645 ?
Te2 Ba2 Ba4 97.12(2) . 2_745 ?
Te2 Ba2 Te10 68.71(2) 2_645 2_645 ?
Te2 Ba2 Te10 140.02(3) . 2_645 ?
Te2 Ba2 Te8 70.33(2) . . ?
Te2 Ba2 Te8 75.28(2) 2_645 . ?
Te2 Ba2 Te12 94.41(2) . 4_575 ?
Te2 Ba2 Te12 129.64(3) 2_645 4_575 ?
Te2 Ba2 Te2 135.56(2) . 2_645 ?
Ba2 Ba4 Ba5 93.474(17) 2_755 . ?
Ba2 Ba4 Ba5 89.612(17) 2_655 . ?
Ba2 Ba4 Ba2 176.21(2) 2_655 2_755 ?
Te9 Ba4 Ba5 85.552(19) 1_655 . ?
Te9 Ba4 Ba5 141.00(2) 2_655 . ?
Te9 Ba4 Ba2 88.94(2) 1_655 2_655 ?
Te9 Ba4 Ba2 93.49(2) 1_655 2_755 ?
Te9 Ba4 Ba2 81.347(19) 2_655 2_755 ?
Te9 Ba4 Ba2 94.87(2) 2_655 2_655 ?
Te9 Ba4 Te9 133.15(2) 2_655 1_655 ?
Te3 Ba4 Ba5 46.334(17) . . ?
Te3 Ba4 Ba2 45.102(17) . 2_655 ?
Te3 Ba4 Ba2 138.42(2) . 2_755 ?
Te3 Ba4 Te9 134.70(3) . 2_655 ?
Te3 Ba4 Te9 75.92(2) . 1_655 ?
Te3 Ba4 Te11 127.09(3) . 3_776 ?
Te3 Ba4 Te14 63.78(2) . . ?
Te15 Ba4 Ba5 87.20(2) . . ?
Te15 Ba4 Ba2 48.294(17) . 2_655 ?
Te15 Ba4 Ba2 129.62(2) . 2_755 ?
Te15 Ba4 Te9 136.65(3) . 1_655 ?
Te15 Ba4 Te9 68.02(2) . 2_655 ?
Te15 Ba4 Te3 68.44(2) . . ?
Te15 Ba4 Te11 83.71(2) . 3_776 ?
Te15 Ba4 Te8 82.35(2) . 2_655 ?
Te15 Ba4 Te4 140.52(3) . 2_755 ?
Te15 Ba4 Te14 45.96(2) . . ?
Te11 Ba4 Ba5 90.17(2) 3_776 . ?
Te11 Ba4 Ba2 45.938(17) 3_776 2_755 ?
Te11 Ba4 Ba2 131.95(2) 3_776 2_655 ?
Te11 Ba4 Te9 138.90(3) 3_776 1_655 ?
Te11 Ba4 Te9 58.68(2) 3_776 2_655 ?
Te11 Ba4 Te14 64.51(2) 3_776 . ?
Te10 Ba4 Ba5 47.396(17) 1_655 . ?
Te10 Ba4 Ba2 50.592(17) 1_655 2_755 ?
Te10 Ba4 Ba2 133.09(2) 1_655 2_655 ?
Te10 Ba4 Te9 129.43(3) 1_655 2_655 ?
Te10 Ba4 Te9 72.44(2) 1_655 1_655 ?
Te10 Ba4 Te3 88.18(2) 1_655 . ?
Te10 Ba4 Te15 128.30(3) 1_655 . ?
Te10 Ba4 Te11 74.78(2) 1_655 3_776 ?
Te10 Ba4 Te8 144.65(3) 1_655 2_655 ?
Te10 Ba4 Te4 81.97(2) 1_655 2_755 ?
Te10 Ba4 Te14 82.45(2) 1_655 . ?
Te8 Ba4 Ba5 133.84(2) 2_655 . ?
Te8 Ba4 Ba2 127.18(2) 2_655 2_755 ?
Te8 Ba4 Ba2 50.944(18) 2_655 2_655 ?
Te8 Ba4 Te9 74.09(2) 2_655 2_655 ?
Te8 Ba4 Te9 72.61(2) 2_655 1_655 ?
Te8 Ba4 Te3 88.41(2) 2_655 . ?
Te8 Ba4 Te11 132.60(3) 2_655 3_776 ?
Te8 Ba4 Te4 81.62(2) 2_655 2_755 ?
Te8 Ba4 Te14 126.59(3) 2_655 . ?
Te4 Ba4 Ba5 128.88(2) 2_755 . ?
Te4 Ba4 Ba2 132.36(2) 2_755 2_655 ?
Te4 Ba4 Ba2 46.320(17) 2_755 2_755 ?
Te4 Ba4 Te9 70.42(2) 2_755 1_655 ?
Te4 Ba4 Te9 72.95(2) 2_755 2_655 ?
Te4 Ba4 Te3 146.33(3) 2_755 . ?
Te4 Ba4 Te11 81.14(2) 2_755 3_776 ?
Te4 Ba4 Te14 144.94(3) 2_755 . ?
Te14 Ba4 Ba5 49.117(17) . . ?
Te14 Ba4 Ba2 100.56(2) . 2_755 ?
Te14 Ba4 Ba2 79.82(2) . 2_655 ?
Te14 Ba4 Te9 93.60(2) . 2_655 ?
Te14 Ba4 Te9 132.84(3) . 1_655 ?
Ba4 Te9 Ba4 166.63(2) 2_645 1_455 ?
In2 Te9 Ba4 89.60(3) . 1_455 ?
In2 Te9 Ba4 87.86(3) . 2_645 ?
Ge2 Te9 Ba4 84.39(3) 1_455 2_645 ?
Ge2 Te9 Ba4 108.77(4) 1_455 1_455 ?
Ge2 Te9 In2 90.72(4) 1_455 . ?
Ba5 Te3 Ba4 85.42(2) . . ?
Ba6 Te3 Ba5 87.75(2) . . ?
Ba6 Te3 Ba4 159.52(3) . . ?
Ba2 Te3 Ba5 158.06(3) 2_655 . ?
Ba2 Te3 Ba6 93.12(2) 2_655 . ?
Ba2 Te3 Ba4 86.21(2) 2_655 . ?
Ge1 Te3 Ba5 113.82(4) . . ?
Ge1 Te3 Ba6 86.71(4) . . ?
Ge1 Te3 Ba2 88.11(4) . 2_655 ?
Ge1 Te3 Ba4 113.70(4) . . ?
Ba3 Te15 Ba1 85.85(2) 1_565 1_565 ?
Ba3 Te15 Ba2 173.25(3) 1_565 2_655 ?
Ba3 Te15 Ba4 96.94(3) 1_565 . ?
Ba2 Te15 Ba1 91.78(2) 2_655 1_565 ?
Ba4 Te15 Ba1 173.36(3) . 1_565 ?
Ba4 Te15 Ba2 84.77(2) . 2_655 ?
Te14 Te15 Ba1 117.36(3) . 1_565 ?
Te14 Te15 Ba3 68.99(2) . 1_565 ?
Te14 Te15 Ba2 117.63(3) . 2_655 ?
Te14 Te15 Ba4 69.27(2) . . ?
Ba1 Te11 Ba3 84.56(2) 3_666 3_766 ?
Ba1 Te11 Ba4 174.60(3) 3_666 3_776 ?
Ba3 Te11 Ba4 93.97(2) 3_766 3_776 ?
Ba2 Te11 Ba1 95.58(3) 4_576 3_666 ?
Ba2 Te11 Ba3 174.11(3) 4_576 3_766 ?
Ba2 Te11 Ba4 85.34(2) 4_576 3_776 ?
Te12 Te11 Ba1 69.86(3) . 3_666 ?
Te12 Te11 Ba3 114.89(3) . 3_766 ?
Te12 Te11 Ba2 70.53(3) . 4_576 ?
Te12 Te11 Ba4 115.39(3) . 3_776 ?
Ba5 Te10 Ba2 147.89(3) 1_455 2_655 ?
Ba6 Te10 Ba5 85.15(2) . 1_455 ?
Ba6 Te10 Ba2 87.28(2) . 2_655 ?
Ba6 Te10 Ba4 147.06(3) . 1_455 ?
Ba4 Te10 Ba5 86.29(2) 1_455 1_455 ?
Ba4 Te10 Ba2 83.31(2) 1_455 2_655 ?
In2 Te10 Ba5 115.00(3) . 1_455 ?
In2 Te10 Ba6 116.24(3) . . ?
In2 Te10 Ba2 96.32(3) . 2_655 ?
In2 Te10 Ba4 96.19(3) . 1_455 ?
Ba1 Te8 Ba3 83.57(2) . 1_455 ?
Ba1 Te8 Ba2 88.30(2) . . ?
Ba1 Te8 Ba4 150.91(3) . 2_645 ?
Ba3 Te8 Ba2 154.52(3) 1_455 . ?
Ba4 Te8 Ba3 93.22(2) 2_645 1_455 ?
Ba4 Te8 Ba2 82.29(2) 2_645 . ?
In2 Te8 Ba1 115.56(3) . . ?
In2 Te8 Ba3 111.28(3) . 1_455 ?
In2 Te8 Ba2 94.02(3) . . ?
In2 Te8 Ba4 92.61(3) . 2_645 ?
Ba3 Te4 Ba1 85.80(2) . . ?
Ba3 Te4 Ba2 168.21(3) . . ?
Ba3 Te4 Ba4 95.41(3) . 2_745 ?
Ba2 Te4 Ba1 90.13(2) . . ?
Ba2 Te4 Ba4 86.03(2) . 2_745 ?
Ba4 Te4 Ba1 166.58(3) 2_745 . ?
Ge2 Te4 Ba1 106.77(4) . . ?
Ge2 Te4 Ba3 86.96(4) . . ?
Ge2 Te4 Ba2 104.81(4) . . ?
Ge2 Te4 Ba4 86.64(4) . 2_745 ?
Ba5 Te13 Ba5 98.05(2) 3_776 . ?
Ba5 Te13 Ba6 82.92(2) . . ?
Ba5 Te13 Ba6 178.30(3) 3_776 . ?
Ba6 Te13 Ba5 82.70(2) 3_676 3_776 ?
Ba6 Te13 Ba5 177.03(3) 3_676 . ?
Ba6 Te13 Ba6 96.25(2) 3_676 . ?
Te14 Te13 Ba5 65.58(2) . . ?
Te14 Te13 Ba5 65.40(2) . 3_776 ?
Te14 Te13 Ba6 113.92(3) . . ?
Te14 Te13 Ba6 112.35(3) . 3_676 ?
Te12 Te13 Ba5 114.30(3) . . ?
Te12 Te13 Ba5 115.94(3) . 3_776 ?
Te12 Te13 Ba6 67.72(2) . 3_676 ?
Te12 Te13 Ba6 64.74(2) . . ?
Te12 Te13 Te14 178.60(4) . . ?
Ba1 Te1 Ba6 167.35(3) . . ?
In1 Te1 Ba1 86.13(3) . . ?
In1 Te1 Ba6 88.52(3) . . ?
Ge1 Te1 Ba1 108.34(4) . . ?
Ge1 Te1 Ba6 83.50(3) . . ?
Ge1 Te1 In1 94.67(4) . . ?
Ba5 Te14 Ba5 97.04(2) 3_776 . ?
Ba3 Te14 Ba5 160.87(3) 1_565 . ?
Ba3 Te14 Ba5 81.51(2) 1_565 3_776 ?
Ba3 Te14 Ba4 92.89(2) 1_565 . ?
Ba4 Te14 Ba5 82.50(2) . . ?
Ba4 Te14 Ba5 161.54(3) . 3_776 ?
Te15 Te14 Ba5 127.92(3) . . ?
Te15 Te14 Ba5 126.56(3) . 3_776 ?
Te15 Te14 Ba3 64.77(2) . 1_565 ?
Te15 Te14 Ba4 64.76(2) . . ?
Te15 Te14 Te13 106.48(3) . . ?
Te13 Te14 Ba5 64.52(2) . 3_776 ?
Te13 Te14 Ba5 64.54(2) . . ?
Te13 Te14 Ba3 129.68(3) . 1_565 ?
Te13 Te14 Ba4 129.91(3) . . ?
Ba3 Te5 Ba5 165.60(3) . . ?
In1 Te5 Ba5 86.19(3) . . ?
In1 Te5 Ba3 90.15(3) . . ?
Ge2 Te5 Ba5 110.23(4) . . ?
Ge2 Te5 Ba3 83.98(3) . . ?
Ge2 Te5 In1 95.96(4) . . ?
Ba1 Te12 Ba6 161.13(3) 3_666 3_676 ?
Ba6 Te12 Ba1 82.54(2) . 3_666 ?
Ba6 Te12 Ba6 95.11(2) . 3_676 ?
Ba6 Te12 Ba2 159.32(3) . 4_576 ?
Ba2 Te12 Ba1 90.12(2) 4_576 3_666 ?
Ba2 Te12 Ba6 85.61(2) 4_576 3_676 ?
Te11 Te12 Ba1 64.51(2) . 3_666 ?
Te11 Te12 Ba6 128.37(3) . 3_676 ?
Te11 Te12 Ba6 128.30(3) . . ?
Te11 Te12 Ba2 63.55(2) . 4_576 ?
Te11 Te12 Te13 105.43(3) . . ?
Te13 Te12 Ba1 130.53(3) . 3_666 ?
Te13 Te12 Ba6 63.66(2) . 3_676 ?
Te13 Te12 Ba6 66.51(2) . . ?
Te13 Te12 Ba2 130.68(3) . 4_576 ?
Ba2 Te2 Ba1 83.39(2) 2_655 2_655 ?
Ba2 Te2 Ba1 85.76(2) . 2_655 ?
Ba2 Te2 Ba2 167.85(3) . 2_655 ?
In2 Te2 Ba1 127.44(3) . 2_655 ?
In2 Te2 Ba2 94.63(3) . . ?
In2 Te2 Ba2 96.30(3) . 2_655 ?
Ge1 Te2 Ba1 141.02(4) . 2_655 ?
Ge1 Te2 Ba2 103.13(4) . . ?
Ge1 Te2 Ba2 82.17(3) . 2_655 ?
Ge1 Te2 In2 90.10(4) . . ?
Ba5 Te7 Ba1 145.97(3) 3_766 . ?
Ba5 Te7 Ba6 85.34(2) 3_766 3_666 ?
Ba5 Te7 Ba3 83.77(2) 3_766 . ?
Ba1 Te7 Ba6 85.46(2) . 3_666 ?
Ba1 Te7 Ba3 85.52(2) . . ?
Ba6 Te7 Ba3 145.47(3) 3_666 . ?
In1 Te7 Ba5 123.20(3) . 3_766 ?
In1 Te7 Ba1 89.19(3) . . ?
In1 Te7 Ba6 121.85(3) . 3_666 ?
In1 Te7 Ba3 91.26(3) . . ?
Ba5 Te6 Ba1 145.73(3) . 3_666 ?
Ba6 Te6 Ba5 85.52(2) . . ?
Ba6 Te6 Ba1 84.09(2) . 3_666 ?
Ba3 Te6 Ba5 84.60(2) 3_766 . ?
Ba3 Te6 Ba1 84.30(2) 3_766 3_666 ?
Ba3 Te6 Ba6 142.92(3) 3_766 . ?
In1 Te6 Ba5 87.78(3) . . ?
In1 Te6 Ba1 125.16(3) . 3_666 ?
In1 Te6 Ba6 92.31(3) . . ?
In1 Te6 Ba3 122.85(3) . 3_766 ?
Te1 In1 Te5 107.38(4) . . ?
Te7 In1 Te1 104.72(4) . . ?
Te7 In1 Te5 102.30(4) . . ?
Te7 In1 Te6 132.30(4) . . ?
Te6 In1 Te1 101.60(3) . . ?
Te6 In1 Te5 106.80(4) . . ?
Te10 In2 Te9 97.54(3) . . ?
Te10 In2 Te8 151.16(4) . . ?
Te10 In2 Te2 95.32(3) . . ?
Te8 In2 Te9 99.71(3) . . ?
Te8 In2 Te2 97.77(3) . . ?
Te2 In2 Te9 115.69(4) . . ?
Te9 Ge2 Te5 111.07(5) 1_655 . ?
Te4 Ge2 Te9 113.04(5) . 1_655 ?
Te4 Ge2 Te5 111.70(5) . . ?
Ge1 Ge2 Te9 107.23(6) . 1_655 ?
Ge1 Ge2 Te4 108.16(6) . . ?
Ge1 Ge2 Te5 105.18(6) . . ?
Te3 Ge1 Te1 111.74(5) . . ?
Te3 Ge1 Te2 112.44(5) . . ?
Te1 Ge1 Te2 112.29(5) . . ?
Ge2 Ge1 Te3 103.12(6) . . ?
Ge2 Ge1 Te1 107.70(6) . . ?
Ge2 Ge1 Te2 109.00(6) . . ?

_olex2_submission_special_instructions 'No special instructions were received'
_exptl_crystal_recrystallization_method 'From the Melt'
